Review Article | Open Access
Antonio Chica, "Zeolites: Promised Materials for the Sustainable Production of Hydrogen", International Scholarly Research Notices, vol. 2013, Article ID 907425, 19 pages, 2013. https://doi.org/10.1155/2013/907425
Zeolites: Promised Materials for the Sustainable Production of Hydrogen
Zeolites have been shown to be useful catalysts in a large variety of reactions, from acid to base and redox catalysis. The particular properties of these materials (high surface area, uniform porosity, interconnected pore/channel system, accessible pore volume, high adsorption capacity, ion-exchange ability, and shape/size selectivity) provide crucial features as effective catalysts and catalysts supports. Currently, new applications are being developed from the considerable existing knowledge about these important and remarkable materials. Among them, those applications related to the development of processes with less impact on the environment (green processes) and with the production of alternative and cleaner energies are of paramount importance. Hydrogen is believed to be critical for the energy and environmental sustainability. It is a clean energy carrier which can be used for transportation and stationary power generation. In the production of hydrogen, the development of new catalysts is one of the most important and effective ways to address the problems related to the sustainable production of hydrogen. This paper explores the possibility to use zeolites as catalysts or supports of catalysts to produce hydrogen from renewable resources. Specifically, two approaches have been considered: reforming of biomass-derived compounds (reforming of bioethanol) and water splitting using solar energy. This paper examines the role of zeolites in the preparation of highly active and selective ethanol steam reforming catalysts and their main properties to be used as efficient water splitting photocatalysts.
1. Zeolites: Composition, Structure, Properties, and Applications
Zeolites were first described in 1756 by the Swedish mineralogist Cronstedt . However, the systematic research efforts on synthetic zeolites were initiated by Barrer in the late 1930s [2, 3]. Barret offered the first classification of zeolites based on molecular size . Inspired by the work of Barrer, researchers at Union Carbide developed synthesis procedures for preparation of the first synthetic zeolites (i.e., zeolites A, X, and Y) that would find industrial applications [5–7].
Initially zeolites were applied as materials for drying and separation substances. Later, with the development of the concept of acid zeolite catalyst, in 1959, they were used as catalysts in the isomerization of hydrocarbons . Previously, Houdry et al.  used them in catalytic cracking of hydrocarbons. Since the development of the first concepts, to date many business processes based on zeolites as catalysts have been implemented. The specialization and knowledge of zeolites have grown so much that the International Zeolite Association (IZA) was founded  and currently there are numerous specialized scientific publications that collect not only the current knowledge about these materials but also their outstanding commercial application.
1.1. Composition and Structure
Zeolites are microporous crystalline aluminosilicates whose chemical composition is defined by the following general formula : where M is a metal cation of valence , and .
Zeolite framework is formed from corner sharing and tetrahedra which define the cavities and channels, in which the cations can be found coordinating to the framework oxygens and/or water molecules. Figure 1 shows the different representations, typical of those used in the literature, of the framework of one zeolite.
The ways to combine each tetrahedron are extremely wide. The structure of the zeolite is defined by its corner sharing tetrahedra of and , and these are called secondary building units (SBUs)  (see Figure 2).
The utility of these constructions is that the angles and distances of zeolites are contained in these SBUs, so the structural characterization of one zeolite could be carried out by examining the SBUs that it contains. There are 16 different SBUs, and the structure of each zeolite can be described using one or more of these SBUs.
In zeolites, the organization of TO4 tetrahedra can result in the formation of rings with different numbers of T atoms (Si, Al). The most common rings are 4-T, 6-T, 8-T, 10-T, and 12-T; however, zeolitic structures containing 14, 18, and 30 member rings have been also synthesized [13–20]. The size of the micropores of the zeolite varies depending on the number of members in the rings, between 4 and 12 Å. On rings, T-O-T angles vary mostly in the range 130°–180°. The flexibility of this angle is one of the most important factors determining the huge variety of existing zeolites.
Zeolites may act as molecular sieves, thus one of their main physical properties is the porosity. The microporous properties of zeolites make them present an extremely large internal surface area in relation to their external surface. Micropores are open to the outside allowing the transference of matter between the intracrystalline space and the surrounding environment.
Tridimensional networks of well-defined micropores can act as reaction channels whose activity and selectivity will be enhanced by introducing active sites. The presence of strong electric fields and controllable adsorption properties within the pores will produce a unique type of catalyst, which by itself can be considered as a catalytic microreactor.
The size of the pores and channels of zeolites ranges between 4 and 12 Å  and the channel system may be mono-, bi-, or three-directional. Table 1 shows the classification of zeolites based on the number of tetrahedrals that form the pores and give access to the intracrystalline space [22–25].
Summarizing, the main properties of zeolites are as follows:(i)high surface area,(ii)molecular dimensions of the pores,(iii)high adsorption capacity,(iv)partitioning of reactant/products,(v)possibility of modulating the electronic properties of the active sites,(vi)possibility for preactivating the molecules when in the pores by strong electric fields and molecular confinement.
Zeolites have a variety of industrial applications, especially as ion exchangers, adsorbents, and chemicals catalysts.
Zeolites as adsorbents are used in processes of separation and purification of gases and liquids due to their ability to adsorb selectively molecules of different size or polarity. They are used in the separation of oxygen from air to remove the water and CO2 from gas streams, separation of the linear branched hydrocarbons, and in the elimination of volatile organic compounds from automobile and industrial exhausted gasses [6, 26–35].
The most important application of zeolites as ion exchangers is the extraction of cations Ca2+ and Mg2+ of domestic and industrial waste water . Sodium zeolite A is used in the formulation of detergents to replace polyphosphates and others highly polluting compounds. They are also used in extraction of NH4+ from waste water  and they have been also used extensively in nuclear waste cleanup (i.e., after the Three Mile Island and Chernobyl nuclear accidents).
Regarding to the use of zeolites as catalysts or catalysts supports, their use is very common in industrial processes of refining, petrochemicals, and fine chemicals. The replacement of conventional catalysts in many processes by zeolites is due to improvements that these materials introduce in the catalytic activity and selectivity.
For the commercial application of zeolites as catalysts together with a good texture-related properties (area, porosity) and a high number of active sites, zeolites must have good thermal stability, since a large part of catalytic processes are conducted at elevated temperatures. Moreover, it is very frequent that the catalysts used in reactions involving hydrocarbons are deactivated by coke deposits formed during the reaction. Thus, they need to be regenerated. The regeneration is conducted by burning the coke at temperatures above 500°C [36–38]. The thermal stability of a zeolite depends on the aluminum content. Al–O bonds are weaker than the Si–O one (Al–O distance is larger than Si–O), therefore the stability depends on aluminum content . Thus, in order to carry out a sufficient number of reaction-regeneration cycles, zeolites with high thermal stability are required, that is, zeolites with Si/Al ≥ 5 . These compositions in some cases can be achieved by direct synthesis (i.e., Beta and ZSM-5 zeolites), and in other cases in which it is not possible by direct synthesis it can be achieved by chemical or hydrothermal treatments of synthesized zeolite (i.e., zeolite Y) [41–43].
The substitution of Si by Al together with the corresponding compensation cations has another additional effect on the properties of the zeolites, hydrophilicity/hydrophobicity . The hydrophilic-hydrophobic character has focused on applications of great practical interest. Thus, the hydrophobic zeolites are able to carry out reactions that require absence of water, without the necessity to remove it from the medium, because the reaction takes place almost entirely inside the zeolite, which being hydrophobic will be water free . For example, silicalite (ZSM-5 structure with Si/Al > 1000)  has very low amount of aluminum, in such a way that its crystals ( g/cc) can float in the water . By contrast, zeolite X, with high Al content, has a pronounced hydrophilic character, which permits separating a mixture of oxygen and nitrogen  due to the higher quadrupole moment of the nitrogen.
The negative charge associated with the tetracoordinated aluminum is compensated by cations that can be easily exchanged for other cations by ion exchange processes . The exchange of cations is favored by the fact that the cations are not covalently bonded to the structure; they are placed inside the zeolite cavities compensating the defect of charge. The size and charge of the exchanged cations are important variables in the zeolite reactivity. Cations of large size will leave small free spaces in the cavities difficulting the entrance of reactants. This effect is very useful in those reactions where the selective control is based on geometric effects [49, 50]. Among the exchangeable cations that can be introduced into the zeolite, the proton occupies a special place. The protons are bonded to an oxygen bridge between one silicon and one aluminum [51, 52]. Due to the presence of channels and cavities of different sizes within the same structure, as well as the existence of nonequivalent positions, there is a paramount importance to predict minimum energy positions, and therefore the location of the exchangeable cations , and especially the localization of the protons that will determine the activity in acid catalyzed reactions.
New scientific applications were considered in the 1980s and 1990s for exploring zeolites as advanced solid state materials. Ozin et al.  considered that zeolites could represent a “new frontier” of solid state chemistry with interesting properties (nanometer dimension window, channel and cavity architecture) for innovative research and development. Among others they consider applications such as: molecular electronics, quantum dots/chains, zeolite electrodes, batteries, nonlinear optical materials, and chemical sensors. Other applications recently reported are related to the use of zeolites as low k dielectric materials for microprocessors .
Future trends in zeolites include (i) discovery of new zeolitic materials, (ii) continuous use in petroleum refining (high octane and reformulated gasoline, processing of heavy crudes, production of diesel, and so forth), (iii) use in the preparation of organic chemical intermediates or end-products, and (iv) use in sustainable processes to produce biocompounds and green fuels.
Considering the future trends, it is quite evident that zeolites are of great interest for the industry, especially due to the potential they present in fields that are of paramount importance for the future of our industrialized society, such as raw material transformation, environmental pollution control, and energy production and storage.
This paper focuses on the application of zeolites for energy production. Specifically, the use of zeolites in the production of hydrogen from renewable energy sources is collected: biomass (ethanol reforming) and solar (water splitting).
2. Zeolites for Hydrogen Production
The future energy economy will have an important role for hydrogen (H2) as a clean and CO2-neutral energy source . Thus, it has been projected as one of the few long-term sustainable clean energy carriers. Currently the synthesis of molecular hydrogen occurs mostly by nonsustainable methods such as steam reforming (SR) of natural gas or gasification of coal, which is associated with the emission of large quantities of greenhouse gases (GHG), especially carbon dioxide (CO2) [57–60]. Thus, to realize the full benefits of a hydrogen economy, increased energy security, diverse energy supply, and reduced air pollution, hydrogen must be produced cleanly and efficiently from available renewable resources. Hydrogen can be produced from renewable resources (e.g., biomass and water) using renewable energy sources (e.g., sunlight, wind, wave, or hydropower) [61–66].
Two important approaches are considered in this paper to produce hydrogen from renewable sources and reduce the CO2 emissions. One approach is to apply reforming methods to biomass-derived compounds, for example, bioethanol. Because biomass consumes atmospheric carbon dioxide (CO2) during growth, it can have a small net CO2 impact compared with fossil fuels. The second approach considers the production of hydrogen by water splitting using solar energy. Hydrogen production by water splitting corresponds to those methods including outside the C-cycle. This process is very attractive due to the potential to use the solar energy which is very abundant.
The use of catalysts to improve the production of hydrogen by reforming of bioethanol and water splitting has been reported. Among them, zeolites seem to have a promised future as catalysts and catalysts supports. Here we will review first the use of different zeolites in the production of hydrogen by ethanol (or bioethanol) steam reforming. We will show the influence that the zeolites have as supports to prepare ethanol reforming catalysts with high activity, selectivity, and stability. Second, we will show the last advances in the use of the zeolites to produce hydrogen by water splitting process and the promised future that these materials have by taking advantage of solar energy.
2.1. Zeolites as Constituents of Catalysts for the Sustainable Production of Hydrogen via Ethanol/Bioethanol Reforming
Among the liquid biomass-derived molecules that can be used as hydrogen source, primary alcohols are interesting compounds because they can be converted to hydrogen by steam reforming using moderate reaction conditions. The most part of the reforming studies related to alcohols from biomass is focused on ethanol. Ethanol is considered an interesting alternative for the sustainable hydrogen production because of (i) its low toxicity; (ii) its low production costs; (iii) the fact that it is a relative clean fuel in terms of composition; (iv) its relatively high hydrogen content; (v) its availability and easiness of handling.
Catalytic hydrogen production from ethanol can be performed by (i) steam reforming (SR), represented by the reaction (2), (ii) partial oxidation (PO), represented by the reaction (3), and (iii) autothermal reforming (ATR), represented by the reaction (4) as follows:
The SR of ethanol, reaction (2), is an endothermic reaction which takes place at temperatures between 673 and 1073 K and with a kinetic slower than the PO reaction. SR operates at lower temperature and produces a higher number of molecules of H2 per molecule of converted ethanol (H2/C2H5OH = 6), thus the overall efficiency of this reaction is higher than that obtained by PO processes.
The PO of ethanol, reaction (3), occurs between 973 and 1273 K. It is an exothermic reaction. It has several advantages: allows working with adiabatic reactors without the necessity to supply external heat and the kinetics is rapid. Obtaining hydrogen from bioethanol by reaction PO is an option that has been rarely investigated, because it would involve the separation of water included in raw bioethanol, which would mean a high energy cost.
The third option combines the advantages of both approaches, SR and PO. This option includes the simultaneous reaction of ethanol with water vapor and oxygen in an oxidative reforming process (autothermal reforming, ATR), reaction (4). The input of the external heat is not necessary since it is generated by introducing small amounts of oxygen. The moles of H2 obtained per mole of ethanol are higher than that in the case of the PO reaction but lower than that in the case of SR.
The choice of the reforming route is based on the type of fuel cell, the demands and volume of the system, and management strategy. Nevertheless, the SR of ethanol has been the most studied route. The amount of published studies on the SR of ethanol is lower than that on hydrocarbons or methanol. Several reviews about the development of catalysts applied to ethanol SR have been published lately [67–70]. Catalytic materials such as metallic oxides (ZnO, MgO, V2O5, Al2O3, TiO2, La2O3, CeO2, SmO3) [71–73], supported metals (Co/Al2O3, Co/La2O3, Co/SiO2, Co/MgO, Co/ZrO2, Co–ZnO, Co/TiO2, Co/V2O5, Co/CeO2, Co/Sm2O3, Co/CeO2–ZrO2, Co/C, Ni/La2O3, Ni/(La2O3–Al2O3), Ni/Al2O3, Ni/MgO, Ni–Cu/SiO2, Ni–Cu/Al2O3, Ni–Cu–K/Al2O3) [74–85], and precious metals supported on oxides (Rh/TiO2, Rh/SiO2, Rh/CeO2, Rh/ZrO2, Rh/Al2O3, Rh/MgO, Rh/Al2O3, Rh/CeO2–ZrO2, Rh–Au/CeO2, Rh–Pt/CeO2, Pd/CeO2, Pt/CeO2, Au/CeO2, Pd/Al2O3, Pt–Pd/CeO2) [86–99] are reported in these reviews.
Thermodynamic analyses have shown that a high conversion of ethanol to hydrogen is possible above 523 K and also that the high water/ethanol molar ratio of raw bioethanol is beneficial to increase hydrogen yield and to decrease the formation of byproducts such as methane, carbon monoxide, and carbon deposition. Table 1 shows a summary of the possible reaction pathways followed by the ethanol during its catalytic SR. The extension in which each reaction takes place over the catalyst will depend on the nature of metal, type of precursor, preparation method, type of support, presence of additives, and operating conditions.
Among them, it is found that support plays an important role in the preparation of highly active and selective ethanol steam reforming catalysts since it helps in the dispersion of metal catalyst and enhances its activity via metal-support interactions. Specifically, it has been found that high surface areas of the support improve the catalytic activity [73, 100], and the particular topology or crystalline structure of one support can affect the metal dispersion of the metallic particles improving their stability against sinterization [101, 102]. Taking this into account, the singular structure of zeolites would make these materials attractive to be used as supports for dispersing active metal phases [102–105].
Campos-Skrobot et al.  reported the first work in the steam reforming of ethanol using zeolites as support. Specifically, they studied the Y-zeolite exchanged with Na. According to the results reported by these authors, the NaY zeolite had the prime function of increasing the surface area, aiming higher reforming reaction efficiency. Potassium and rhodium were added to NaY zeolite in order to improve reforming performance. They found that the addition of Rh and K allowed to prepare an ethanol steam reforming catalyst with high activity and H2 selectivity. Best conversion values were achieved for higher H2O/ethanol ratio and higher reagent flow. They also verified that reagent flow has greater influence on hydrogen yield than K addition. They concluded that NaY zeolite-supported Rh can be considered promising catalyst for ethanol steam reforming, when compared with other existing studies.
Chica et al. [102, 105] also studied zeolitic materials as support of catalyst for the SR of bioethanol. They used two delaminated zeolites (ITQ-2 and ITQ-18) with high external surface area (835 and 611 m2/g, resp.) to support Ni and Co.
ITQ-2 delaminated zeolite consists of thin sheets of 2.5 nm in height presenting a hexagonal array of “cups” (0.7 nm × 0.7 nm) that penetrate into the sheet from both sides connected by a double 6-member ring (MR) window (Figure 3) . ITQ-18 is another delaminated zeolite which has been obtained by expanding and exfoliating a laminar precursor of NU-6 zeolite  (Figure 4). The singular structure of these delaminated zeolites, and particularly the very high and well-defined external surface area, makes these materials very attractive to be used as supports for dispersing active metal phases.
Ni and Co were supported on pure silica ITQ-2 and Co on ITQ-18 with low aluminum content (Si/Al = 100). For comparison reasons, catalysts based on amorphous silica containing the same amount of Co and Ni (20 wt.%) were also prepared. High catalytic activity, selectivity, and stability (again coke deposition) were reported for the delaminated zeolite-based catalysts. The excellent catalytic performance exhibited was attributed to the combination of three effects. It was attributed first to the absence or very low concentrations of acid sites in the delaminated ITQ-2 and ITQ-18 zeolites, respectively. The absence of acid sites would help to decrease the dehydration reaction that leads to the formation of ethylene and subsequent formation of coke, the main causative of the catalyst deactivation. It was attributed second to its high external surface, which can provide a large surface for coke deposition and help to slow down the deactivation effects, and third to the especial structure of these delaminated zeolites formed by array of “cups” distributed along of sheets (see Figures 3 and 4), which can provide an excellent position for the stabilization of the Ni and Co metal particles improving their dispersion and preventing their agglomeration during the reduction and reaction stages. An important conclusion was that while an amorphous support such as SiO2 leads to Co and Ni-based catalysts with low stability, the use of delaminated zeolites, with a crystalline structure, allowed to prepare a much more stable bioethanol steam reforming catalyst.
In the before reported studies, zeolites are acting as simple supports for metals for ethanol steam reforming [102–105]. However, since zeolites exhibit functional properties such as ion exchange, the charge state of the metal could affect the SR of ethanol. In this line, Inokawa et al.  compared the ethanol reforming properties of zeolite Y supporting transition metals and encapsulating transition metal cations.
They studied the catalytic activity of conventional zeolite Y with a Si/Al ratio of 2.75, loaded with Ni and Co and their cations. The results obtained suggest that transition metals selectively enhanced the dehydrogenation of ethanol. In addition, the incorporated transition metal cations by ion exchange led to the production of mainly C2H4 during ethanol steam reforming, indicating that the presence of the cations accelerates the dehydration of ethanol. Thus, the presence of transition metal cations in zeolite Y seems to have a significant influence on the ethanol reforming reaction. These authors suggest that conventional zeolites supporting transition metals are more attractive for industrial applications than zeolites with a high Si/Al ratio supporting noble metals, due to advantages of cost and availability, although the H2 yields produced by Y zeolite containing Co and Ni cations were inferior to that for zeolite Y supporting Rh . In addition, they think that H2 production from ethanol using zeolites with low or medium Si/Al ratios supporting transition metals such as Co and Ni could be improved by the removal of the metal cations within the zeolites.
One important factor affecting the stability of steam reforming catalysts is the formation of carbonaceous deposits. These deposits can block the active sites and finally encapsulate the metallic particles deactivating the catalyst completely. Therefore, the stability of the catalysts is directly related to their tendency to form carbon. The coke formation on the catalysts during reforming of ethanol is due to the imbalance between their formation and consumption reactions (Table 2). This balance formation/consumption is determined by the reaction conditions and especially by the selected catalyst composition: active phase and support.
In order to reduce the coke formation over zeolite-based catalysts and increase the ethanol SR activity at low temperature, Kwak et al.  prepared MgO/zeolite Y catalysts loaded with bimetallic Ni-Ga. The impregnation of Ga between the Ni and Mg components led to significantly higher reforming activity compared to the conventional Ni/Mg/zeolite Y catalyst. The main products from steam reforming over the Ni/Ga/Mg/zeolite Y catalyst were only H2 and CH4 at above 550°C, and the catalytic performances depended on the amount of Ga. H2 production and ethanol conversion were maximized over Ni(10)/Ga(30)/Mg(30)/zeolite Y at 973 K, ethanol : H2O = 1 : 3, and a gas hourly space velocity (GHSV) of 6740 h−1. This high performance was maintained for up to 59 h.
These authors also studied the deactivation of these catalysts. They found that deactivation was largely retarded in the zeolite-based catalyst containing Ga compared to that of the catalyst without Ga. The authors reported that after 60 h the XRD peaks of the carbon and Ni metal were too enlarged while the other peaks assigned to metal or metal oxides species were very small (Figure 5). The improved stability at the slower deactivation rate achieved with the Ni/Ga sample could not be unequivocally attributed to carbon formation. The simultaneous addition of Ni/Ga could also have depressed the sintering between the Ni and the support, contributing to retard of the catalytic deactivation.
It is clear that basicity decreases significantly the formation of coke since it contributes to the inhibition of side reactions that would lead to the formation of coke precursors (Table 2). In this sense, Inokawa et al.  studied the ethanol steam reforming over Ni supported on zeolite Y with basicity controlled by the exchange of alkali cations. As a result, it was found that the exchange of Na+ for K+ and Cs+ affected not only characteristics of the zeolites such as adsorption and basicity but also those of Ni, such as reducibility and catalytic activity. Ion exchange mainly brought an increase of basic sites, which were slightly strengthened. It was found that Ni species on the Cs-Y zeolite were reduced at a lower temperature than Na-Y zeolite. H2 production at 573 K was improved in the order of Ni/Na-Y < Ni/K-Y < Ni/Cs-Y, according to the size of the cation in the zeolite and the amount of basic sites. Improvement of the catalytic performance was considered to be due to the increase of basic sites, which weaken the OH bond of ethanol adsorbed on the zeolite. In terms of elementary reactions, the dehydrogenation reaction of ethanol was accelerated by the basicity of the zeolite, whereas the dehydration reaction that produces ethylene was inhibited.
The basicity of the zeolite was found to be effective for the inhibition of coke deposition, because Ni/Cs-Y with higher H2 production than Ni/Na-Y also exhibited higher resistance to carbon deposition. In summary, an increase of the zeolite basicity by cation exchange can selectively promote the dehydrogenation of ethanol by Ni on the zeolite and improve H2 production and resistance to carbon deposition.
Ni and Co have been the active sites more studied in the SR of ethanol using zeolites as support. Nevertheless, other metals as Sn have been also found actives. Lee et al.  studied the production of hydrogen using Y zeolite promoted with Sn and K. They studied the effects of the Sn and K presence on the H2 production and on the catalytic deactivation. They reported that the Sn component played an important role in the oxidation of the feed gases during ethanol reforming, while the addition of the K depressed the formation of CH4 or others hydrocarbon intermediates. Based on the results of H2-TPR and NH3-TPD, they suggest that the reduction of Sn oxides (Sn4+ to Sn0) on SnO2-K2O/Y catalyst at low temperatures easily occurs compared to conventional Ni/γ-Al2O3 catalysts. In addition, the acidity of the Ni/γ-Al2O3 catalyst induced by the existing Al is higher than that presented in the SnO2-K2O/Y catalyst. Thus, the condensation of ethanol on the last catalyst is more difficult and consequently the formation of the coke is lower, and eventually the higher activity over SnO2-K2O/ZY catalyst is maintained.
Considering all the above mentioned, it seems that the use of zeolites as metal support to prepare active and stable reforming catalyst to produce hydrogen could be an attractive option since they have a high external surface area and can be prepared with neutral behaviors if they synthesized all silica, with high Si/Al ratios or exchanged with alkaline metals. However, pore opening of zeolites can limit their application to the reforming of large molecules. Thus, mesoporous molecular sieves with size-tunable mesopores have attracted a great deal of attention because of their controllable structure and composition [110, 111]. However, unlike zeolites, the wall of the mesoporous is amorphous, not crystalline. Therefore, mesoporous aluminosilicates cannot exhibit the excellent catalytic properties unlike acidic zeolites. Moreover, their hydrothermal stability is especially low. To overcome this problem, one strategy has been the generation of mesoporosity on zeolites [112–114]. The presence of mesopores in the crystalline of the zeolite would be equivalent to increasing the external surface of the zeolites making a larger number of pore openings accessible to the large reactants [115–121]. On the other hand, the presence of mesoporous could improve the diffusion affecting the ion exchange processes and catalytic reaction [122–129]. Although ethanol is a small molecule from biomass processing, most part of the molecules from biomass susceptible to be reformed are large (i.e., glycerin, sugars, cellulose, lignin, hemicellulose, and so forth), making the mesopore-modified zeolites an attractive material to prepared hydrothermally stable steam reforming catalysts. In this line, da Costa Serra et al.  studied the effect of mesopores-modified mordenite zeolite promoted with Ni in the steam reforming of bioethanol. They reported the alkaline treatment of a commercial mordenite to generate mesoporosity (Figure 6). The idea was to generate mesoporosity in the commercial mordenite zeolite in order to improve the exchange of alkaline cation (to remove the acidity) and create good positions for the incorporation and stabilization of Ni metallic particles (active sites for steam reforming of bioethanol). They found that reforming activity of catalyst based on mesopores-modified mordenite was significantly higher than that shown by the commercial one (without mesopores). The lower size of the Ni metallic particles supported on mesopores-modified mordenite were the main factor responsible for this high activity. H2 selectivity and catalytic stability were also found higher for the mesopore-modified material. They reported that the formation of coke precursors (favored by acid sites) and the subsequent deposition of carbon was lower in the mesopore-modified mordenite. This effect is explained by the generated mesoporosity, which would improve first the Na exchange and thus, the neutralization of the acid sites, and second the diffusion of the reactants and products, avoiding the blockage of micropores. Indeed, for the same Na exchange conditions, the amount of Na exchanged was found higher in the mesopores-modified mordenite (4.2 wt.% against 2.9 wt.% for original mordenite), suggesting that the presence of mesopores would improve the exchange of protons (responsible of acid sites) by sodium cations. On the other hand, they observed a higher enlargement of the Ni metallic particles supported on not treated mordenite (without mesopores), suggesting that generated mesoporosity could be contributing to the generation of good position for the incorporation and stabilization of Ni metallic particles, avoiding or decreasing the Ni sinterization and thus, improving the catalytic activity and stability.
All the works mentioned above have been centered in the reforming of ethanol or bioethanol in gas phase. Nevertheless, in the literature the use of zeolites in the reforming of ethanol in liquid phase is also reported. Aqueous phase reforming (APR) has been recently reported by Dumesic et al. [131–133]. This process operates at low temperatures (<573 K), at which the WGS reaction is also thermodynamically favored, making it capable of producing hydrogen with high yields. The low reaction temperature minimizes the decomposition reactions and, hence, avoids carbonization and catalyst deactivation. Tang et al.  studied the feasibility of platinum-loaded NaY zeolite catalysts for APR of methanol and ethanol. The feasibility of APR of ethanol was demonstrated on the Pt/NaY catalysts. The results were compared with the data on Pt/γ-Al2O3 catalysts. At 538 K, the 0.5 wt % Pt/NaY achieved higher H2 selectivity and lower alkane selectivity than the 3 wt % Pt/γ-Al2O3 catalyst with similarly high ethanol conversion of ~97% on both catalysts. The zeolite-based catalysts, with the advantages of high activity, reduced use of precious metal, and low cost of zeolite materials, deserve further investigations. They report that research is ongoing into the effect of substrate properties on the catalytic performance of platinum catalysts in APR reactions.
2.2. Zeolites as Constituents of Photocatalysts for the Sustainable Production of Hydrogen via Water Splitting
2.2.1. Solar Energy and Water Splitting Reaction
The incidence of solar energy on the surface of the earth (180.000 TW) by far exceeds all human energy needs . Thus, it is easy to understand that the solar energy could be considered one of the most important renewable energy sources potentially available on earth.
Undoubtedly, solar energy is the largest renewable carbon-free resource amongst all other renewable energy options. However, to make use this energy by the currently human technology, solar energy must be captured, converted, and stored in order to assure a continuous supply of energy and to overcome the diurnal cycle and the intermittency of the terrestrial solar resource.
Among the different energy carriers capturing the solar energy, hydrogen from photocatalytic water splitting is considered as one of the most promised carriers since it allows storing solar energy in the form of chemical energy and makes available solar energy for 24 hours a day, 7 days a week.
In the photocatalytic water splitting, hydrogen is produced from water using sun light and specialized semiconductors. The semiconductor uses light energy to directly dissociate water molecules into hydrogen and oxygen. The water splitting takes place when the semiconductor is irradiated with light in the presence of an electron donor and acceptor, oxidizing OH− ions to produce O2 and reducing H+ ions to H2. Specifically, the electrons in the valence band of the photocatalyst are excited to the conduction band, while the holes are left in the valence band. This, therefore, creates the negative-electron (e−) and positive-hole (h+) pairs. This stage is referred to the semiconductor’s “photo-excited” state, and the energy difference between the valence band and the conduction band is known as the “band gap.” This must correspond to the wavelength of the light for it to be effectively absorbed by the photocatalyst. After photoexcitation, the excited electrons and holes separate and migrate to the surface of the photocatalyst. In the photocatalytic water-splitting reaction, they are used as a reducing agent and oxidizing agent to produce H2 and O2, respectively. A schematic representation of the principle of the photocatalytic system for water is shown in Figure 7 . As it can be seen, first, that O–H bonds of two water molecules need to be broken with the simultaneous formation of one O=O double bond as follows :
Since this reaction requires a high oxidizing potential, 1.23 V versus NHE (normal hydrogen electrode) (pH = 0), the top level of valence band has to be more positive than this potential, so that the photogenerated holes have enough energy to oxidize water. This reaction releases four protons (H+) and four electrons (e−), which need to be combined to form two H2 molecules, as follows : Therefore, the conduction band of the semiconductor has to be more negative than water reduction potential (0 V versus NHE (pH = 0)). Thus, water molecules are oxidized by the holes to form O2 and are reduced by the electrons to form H2 for overall water splitting. Therefore, the theoretical minimum band gap for water splitting is 1.23 eV that corresponds to light wavelength of about 1000 nm.
2.2.2. Semiconductors and Zeolites for Water Splitting
Currently, the photocatalytic water splitting over semiconductor materials is an area of great interest due to the potential of hydrogen as a clean-energy fuel source. Since the initial works of Fujishima and Honda , who discovered that water can be photoelectrochemically decomposed into hydrogen and oxygen using a semiconductor (TiO2) electrode under UV irradiation, an extensive variety of materials (TiO2, CdS, ZnO, ZrO2, titanates, niobates, and tantalates) [139–151] have been reported to be effective for the photocatalytic decomposition of water.
Initial efforts in this area involved large bandgap ( eV) semiconductors that used only UV light. Currently, the most important efforts are being focused on using visible light as the energy source [152–170] as the ultimate goal to produce hydrogen fuel using solar energy. While the overall redox potential of the reaction is only −1.23 eV (1000 nm) at pH 7, the crucial reaction for hydrogen production is believed to be the initial one-electron transfer to H+ ion where V at pH 7, which falls energetically within the visible region of light.
Taking into account the basic mechanism and reactions of photocatalytic water splitting process, the photocatalysts should meet several characteristics with respect to semiconducting and electrochemical properties [171–175] as follows: (1) narrow band gap () and band edge potentials suitable for overall water splitting to be activated under visible light, (2) successive separation of photo-excited electrons from reactive holes, (3) minimum energy losses associated with charge transport and recombination of photo-excited charges, (4) corrosion and photocorrosion resistivity in aqueous mediums, (5) facilitated electron transfer properties from photocatalyst surface to water, and (6) low production cost.
To meet part of the above mentioned expectations, extensive studies have been performed based on the use of support where effective photocatalysts have been impregnated [176–183]. The major incentives for implementing the supported photocatalyst idea are (1) inhibition of the back electron transfer as limiting parameter in redox systems, (2) taking advantage of nanosized semiconductors while using them in easily separable microsized level of the support, (3) utilizing the support to add more solid chemical promoters, and (4) structural and chemical characteristics of the support by itself.
Among the different supports used to prepare efficient water splitting photocatalysts, zeolites are presented as promising materials. Zeolites exhibit high surface area, unique nanoscaled porous structure, and ion exchange properties which can be used in the design of highly efficient photocatalysts . Unique photocatalytic properties, which cannot be realized in normal catalytic systems, have been observed recently in such modified spaces [185–190]. It is important to note that zeolites can also provide specific photophysical properties such as the control of charge transfer and electron transfer processes [191–194] which is very important in photocatalytic reactions.
There are several advantages that zeolites afford as support or host of semiconductor particles. For example, the pore sizes of the host support material control the resulting particle size of the supported semiconductor. Particle size is a crucial factor in the dynamics of electron/hole recombination processes, especially in semiconductor nanomaterials, and that the movement of electrons and holes is primarily governed by the well-known quantum confinement . Generally, a decrease in particle size could be expected to lead to a higher efficiency in photocatalysis [196–201]. This was because the bulk charge recombination of photogenerated electrons and holes, dominant in the well-crystallized large semiconductor particles, was reduced by decreasing particle size. Reduction in particle size could also lead to a larger surface area and an increased available surface active sites [202–204].
Decreasing particle size has a known beneficial effect on catalyst efficiency [205–208]. Furthermore, encapsulation into a porous structure should provide some protection against surface-mediated reactions that corrode the catalyst, as exposed surface area will be limited. In addition, a major factor that limits the efficiency of the most part of the photocatalysts is electron-hole recombination.
The incorporation of photocatalysts into the micropore structure of zeolite in order to prepare nanoparticles is an attempt to improve their photocatalytic activity and photostability. Small nanoparticles show a higher photocatalytic activity compared to the bulk materials due to changes in the surface area, band gap, morphology, and generation of surface defects [209, 210]. In addition, the incorporation of photocatalyst into solid matrices as zeolites is reported to suppress photocorrosion and improve the activity for water reduction. The incorporated nanoparticles, whose sizes are determined by the nanometric size of zeolite cages, show some novel physical properties such as blue shift of optical absorption spectra, increased photooxidation potentials, and third-order nonlinear optical properties. In this line, Sathish et al.  reported the preparation of cadmium sulphide (CdS) nanoparticles by precipitation process using different zeolite matrices as templates (H-Y, HZSM5 and H-β). In this study, the micropores of zeolites were used as molds to prepare nanoparticles of CdS with different sizes. After the removal of zeolite phase, the CdS nanoparticles were used as catalysts for the photocatalytic decomposition of water. The hydrogen evolution rate was found higher than that presented by the bulk samples which correlated quite well with the particle size and surface area.
Of particular interest is the use of zeolites as support, because of the well-defined microporous structure and ion-exchange properties, as was mentioned before. One of the first work reported in the literature about the use of zeolites as support to produce hydrogen by water splitting process was carried out by Fox and Pettit . They studied the photocatalytic hydrogen evolution on zeolite-supported CdS particles modified by surface modification with an appropriate hydrogen evolution catalyst (Pt or ZnS). Particles formed within the zeolite cavities aggregate upon exposure to water, and small clusters were isolated within individual cavities only in nonaqueous solvents at low CdS loading levels (<3%). Sustained hydrogen evolution required the presence of an added sacrificial donor . Platinum deposited on the photoactive CdS surface is exclusively found inside the cavity, where it was inaccessible to large anionic reagents.
Ryu et al.  also studied the water splitting activity of CdS particles supported on several micro- and mesoporous silicas (zeolites: Y and L, mesoporous: SBA-15). Specifically, they studied the hydrogen production from water/ethanol solutions using visible light. All catalysts were active in the photocalytic water splitting with the following order of photoreactivity: zeolite-Y > SBA-15 > zeolite-L. They found that optimization of reaction conditions (i.e., pH, ionic strength, and water-to-alcohol ratios) was critical to achieve a high level of hydrogen production. Preventing loss of CdS during the course of the photoreaction is also paramount to create a stable, long-term use catalyst. Specifically, they found that there was an efficient dispersion of CdS nanoclusters into the cages and micropores of zeolite Y, and the quantum confinement of hydrated CdS increased the reduction potential for the bound proton to hydrogen atom electron transfer, and finally the confined CdS supercluster in a more efficient chromophore in the visible portion of the spectrum.
The water splitting activity with visible light using CdS nanocomposites (quantum-sized (Q-sized) CdS, CdS nanoparticles embedded in zeolite cavities (CdS/zeolite), and CdS quantum dots (Q-CdS) deposited on KNbO3 (CdS/KNbO3 and Ni/NiO/KNbO3/CdS)), was also investigated by Ryu et al. . They reported that the rate of H2 production in alcohol/water mixtures and other electron donors at λ ≥ 400 nm was clearly higher in the the hybrid catalysts, including zeolite-based photocatalyst. The relative order of reactivity as a function of catalyst is Ni(0)/NiO/KNbO3/CdS > Ni(0)/KNbO3/CdS > KNbO3/CdS > CdS/NaY-zeolite > CdS/TiY-zeolite > CdS, while the reactivity order with respect to the array of electron donors is 2-propanol > ethanol > methanol > sulfite > sulfide.
Titanium exchanged zeolites have been also studied in the water splitting reaction. Yue and Khan  were one of the first reporting the use of titano-zeolites to produce hydrogen by water splitting. In their study, the Ti was exchanged and incorporated into the framework of zeolite A. Specifically, they studied the effect of several variables on the photoassisted production of hydrogen over this titanium-exchanged zeolite. During the reaction, oxygen tended to react with titanium ions exchanged on zeolite forming titanium oxides ultimately leaving the zeolite surface thereby creating vacant sites. These vacant sites were occupied by hydrogen, after the absorbed hydrogen was successfully displaced from the zeolite structure by the addition of base.
Zeolites containing titanium in their framework have been also used as support of CdS nanoparticles. In this line, Guan et al. [215, 216] studied the water splitting activity of CdS encapsulated on ETS-4 and ETS-10 titanosilicalite zeolite. They found a stable photocatalytic activity under visible light irradiation (λ > 420 nm) in aqueous solution containing Na2S and Na2SO3 as electron donors. Specifically, the catalytic activity for the zeolite-based photocatalysts was found higher than that for CdS bulk (17.5 and 13,3 μmol H2/h/g catalyst for CdS/ETS-4 and CdS/ETS-10. resp., and, 8.3 μmol H2/h/g catalyst for CdS bulk). These results seem to indicate that the encapsulation of CdS in these titanosilicalite zeolites is effective for separating charge-carries photogenerated in CdS and for improving the activity as well as the stability.
Dubey et al.  reported the use of zeolite Y to prepare highly efficient water splitting catalysts under visible light. They reported the incorporation in the zeolite Y of titanium dioxide (TiO2), heteropolyacid (HPA), and transition metals like cobalt (Co). They got a photocatalyst where the TiO2 was effectively dispersed and stabilized on the zeolite surface. The high efficiency of the composite photocatalyst was explained by the synergetic work of TiO2 with Co and heteropolyacid, which made the material active in visible light for photoreduction of water to hydrogen. They also reported that the aluminosilicate framework of zeolite also contributed towards delayed charge separation.
In the previous studies, zeolites have been used for the separated incorporation of nanoparticles of CdS and titanium (as titanium oxide particles (TiO2) or Ti3+ taking part of the zeolite framework). In this way improved water splitting catalysts were obtained. Recently works carried out by White et al.  report the incorporation of both semiconductors in zeolite Y. They observed improvements in H2 evolution rates of ~300 for CdS/TiO2 zeolite Y over TiO2 zeolite Y and ~18 for CdS/TiO2 zeolite Y over CdS zeolite Y. These improvements exceed colloidal binary systems reported in the literature. On the other hand, improvements in the H2 evolution rate of the ternary system Pt/CdS/TiO2-zeolite Y was not as marked, as compared to the best colloidal ternary systems reported in the literature. They proposed an interesting model to explain the colocalization of the TiO2 and CdS nanoparticles supported on zeolite Y. This model explains quite well the high activity of binary system (CdS/TiO2, zeolite Y) and also why the incorporation of Pt did not improve the catalytic activity of the ternary system (Pt/CdS/YiO2, zeolite Y). The main reason was that Pt needed to be associated only with TiO2 for best H2 evolution, and the zeolite promoted self-assembly did not provide a route for positioning the Pt only on the TiO2 particles. New strategies for the incorporation of Pt will be required in order to promote the association of Pt only with TiO2.
The intense exploitation of fossil fuels to satisfy the globally growing energy demand has caused an increase of CO2 in the atmosphere and, therefore, a significant global warming (green-house effect). Furthermore, the reserves of fossil fuels on earth are finite and no matter how long they will last, a cleaned and renewable energy alternative independent of fossil fuels has to be developed for the future. Hydrogen could be a good option because it exhibits the greatest heating value (39.4 kWh/kg) of all chemical fuels. Its combustion to heat or power is simple and clean. When combusted with oxygen, hydrogen forms water and no pollutants are generated or emitted. About 95% of the hydrogen we use today comes from reforming natural gas. But to realize the full benefits of a hydrogen economy, increased energy security, diverse energy supply, and reduced air pollution, hydrogen must be produced cleanly, efficiently, and affordably from available renewable resources. Thus, renewables are a desired energy source for hydrogen production. However, there are many challenges to produce hydrogen from renewables and probably the major one is developing new catalytic process to produce sustainable hydrogen and reducing the cost to be competitive with the current fuels (gasoline and diesel).
Zeolites are presented as excellent catalysts and support of catalysts due to their very special physicchemical properties. (i)High surface area.(ii)Molecular dimensions of the pores.(iii)High adsorption capacity.(iv)Partitioning of reactant/products.(v)Possibility of modulating the electronic properties of the active sites.(vi)Possibility for preactivating the molecules when in the pores by strong electric fields and molecular confinement.
Currently, new scientific applications have been developed for these materials. Among them, the production of green fuels from renewable sources is the focus of a large part of the research efforts.
Two different routes to produce sustainable hydrogen using zeolites have been described and revised in this paper. One of them is based on the biomass conversion via indirect thermochemical conversion to intermediate products. The indirect thermochemical option is related to the conversion of biomass to biofuels (bioethanol, biodiesel, biogas), followed by catalytic steam reforming of them to hydrogen. An advantage of this approach is that the biofuels, as an intermediate product, have a higher energy density than the biomass feedstock and can be transported more easily. Specifically, this paper has considered the steam reforming of bioethanol.
Renewable bioethanol is an interesting hydrogen source through steam reforming, but its C–C bond promotes parallel reactions, mainly coke and by-products formation. In this way, good ethanol reforming catalysts are still needed. The use of zeolites has been able to improve the catalytic activity, selectivity, and stability of the bioethanol steam reforming catalysts. It has been reported that zeolites play an important role in the preparation of highly active and selective ethanol steam reforming catalysts since they help in the dispersion of metal active sites and enhance their activity via metal-support interactions. Specifically, it has been found that high surface areas of the support improve the catalytic activity and that the particular topology or crystalline structure of one support can affect the metal dispersion of the metallic particles improving their stability against sinterization.
Another interesting option analyzed in this paper, with enormous potential but requiring more development time, has been the photocatalytic decomposition of water using solar energy, which is also called water splitting. In the photolysis of water, solar photons area is used to produce hydrogen directly via electrochemical systems. This method involves the dissociation of water into hydrogen and oxygen directly at the surface of a semiconductor through the irradiation of the semiconductor by solar photons. The photovoltaic semiconductor material acts as a catalyst to produce hydrogen directly at the semiconductor and water interface.
It has been shown that among the different supports used to prepare efficient water splitting, photocatalysts zeolites are presented as promising materials. Zeolites exhibit high surface area, unique nanoscaled porous structure, and ion exchange properties which can be used in the design of highly efficient photocatalyst. In addition, zeolites can also provide specific photophysical properties such as the control of charge transfer and electron transfer processes which are very important in photocatalytic reactions.
It has been seen that there are several advantages that zeolites afford as support or host of semiconductor particles. For example, the pore sizes of the host support material control of the resulting particle size of the supported semiconductor. Semiconductors such as TiO2 and CdS have been incorporated in zeolites in order to improve their photocatalytic activity and photostability. Small nanoparticles of these semiconductors incorporated in zeolites have been reported to show a higher photocatalytic activity compared to the bulk materials due to changes in the surface area, band gap, morphology, and generation of surface defects. In addition, the incorporation of photocatalyst into zeolites helps to suppress photocorrosion and improve the activity for water reduction. Although the studies presented here using zeolites can be considered promising, the major problem to solve would be to find a semiconductor material that had the right photoelectrochemical properties, while being economical and robust enough to withstand the severe chemical and physical environment.
- A. F. Cronstedt, “Rön och beskrifning om en obekant bärg art, som kallas Zeolites,” Akademeins. Handlingar, Stockholm, vol. 18, p. 120, 1756.
- R. M. Barrer and D. A. Ibbison, “Occlusion of hydrocarbons by chabazite and analcite,” Transactions of the Faraday Society, vol. 40, pp. 195–206, 1944.
- R. M. Barrer, “Process for the manufacture of crystalline absorbents,” US Patent 2413134, 1946.
- R. M. Barrer, “Separation of mixtures using zeolites as molecular sieves. I. Three classes of molecular-sieve zeolite,” Journal of the Society of Chemical Industry, vol. 64, p. 130, 1945.
- D. W. Breck, “Crystalline molecular sieves,” Journal of Chemical Education, vol. 41, no. 12, pp. 678–689, 1964.
- R. M. Milton, “Performed zeolites and silicates,” in Molecular Sieves, p. 199, Society of Chemical Industry, London, UK, 1968.
- J. A. Rabo, “Unifying principles in zeolite chemistry and catalysis,” Catalysis Reviews: Science and Engineering, vol. 23, no. 1-2, pp. 293–313, 1981.
- E. M. Flanigen, “Zeolites and molecular sieves. An historical perspective,” in Introduction To Zeolite Science and Practice, H. van Bekkum, E. M. Flanigen, and J. C. Jander, Eds., Studies in Surface Science and Catalysis, pp. 11–37, Elsevier, Amsterdam, The Netherlands, 2nd Completely Revised and Expanded Edition edition, 1991.
- E. Houdry, W. F. Burt, A. E. Pew, and W. A. Peters, “The houdry process,” Oil and Gas Journal, Engineering and Operating Section, vol. 37, pp. 40–45, 1938.
- J. M. Newsman, “The zeolite cage structure,” Science, vol. 231, no. 4742, pp. 1093–1099, 1986.
- W. M. Meier and D. H. Olson, Atlas of Zeolite Structure Types, Structure Commission of the International Zeolite Asociation, 1978.
- C. C. Freyhardt, M. Tsapatsis, R. F. Lobo, K. J. Balkus Jr., and M. E. Davis, “A high-silica zeolite with a 14-tetrahedral-atom pore opening,” Nature, vol. 381, pp. 295–298, 1996.
- R. F. Lobo, M. Tsapatsis, C. C. Freyhardt et al., “Characterization of the extra-large-pore zeolite UTD-1,” Journal of the American Chemical Society, vol. 119, no. 36, pp. 8474–8484, 1997.
- T. Wessels, C. Baerlocher, L. B. McCusker, and E. J. Creyghton, “An ordered form of the extra-large-pore zeolite UTD-1: synthesis and structure analysis from powder diffraction data,” Journal of the American Chemical Society, vol. 121, no. 26, pp. 6242–6247, 1999.
- P. Wagner, M. Yoshikawa, M. Lovallo, K. Tsuji, M. Taspatsis, and M. E. Davis, “CIT-5: a high-silica zeolite with 14-ring pores,” Chemical Communications, no. 22, pp. 2179–2180, 1997.
- A. Burton, S. Elomari, C. Y. Chen et al., “SSZ-53 and SSZ-59: two novel extra-large pore zeolites,” Chemistry, vol. 9, no. 23, pp. 5737–5748, 2003.
- K. G. Strohmaier and D. E. W. Vaughan, “Structure of the first silicate molecular sieve with 18-ring pore openings, ECR-34,” Journal of the American Chemical Society, vol. 125, no. 51, pp. 16035–16039, 2003.
- A. Corma, M. J. Diaz-Cabañas, J. L. Jorda, C. Martinez, and M. Moliner, “High-throughput synthesis and catalytic properties of a molecular sieve with 18- and 10-member rings,” Nature, vol. 443, pp. 842–845, 2006.
- J. L. Sun, C. Bonneau, A. Cantin et al., “The ITQ-37 mesoporous chiral zeolite,” Nature, vol. 458, no. 7242, pp. 1154–1157, 2009.
- M. E. Davis, C. Saldarriaga, C. Montes, J. Garces, and C. Crowdert, “A molecular sieve with eighteen-membered rings,” Nature, vol. 331, no. 6158, pp. 698–699, 1988.
- S. M. Csicsery, “shape-selective catalysis in zeolites,” in Zeolite Chemistry and Catalysis, vol. 171, p. 680, 1976.
- S. M. Csicsery, “Shape-selective catalysis in zeolites,” Zeolites, vol. 4, no. 3, pp. 202–213, 1984.
- E. G. Derouane, “New aspects of molecular shape-selectivity: catalysis by zeolite ZSM-5,” Studies in Surface Science and Catalysis, vol. 5, pp. 5–18, 1980.
- G. E. Derouane, Zeolite Science and the Technology, vol. 80 of NATO ASI Series E, Martinus Nijhoff, The Hague, The Netherlands, 1984.
- A. Corma, “Inorganic solid acids and their use in acid-catalyzed hydrocarbon reactions,” Chemical Reviews, vol. 95, no. 3, pp. 559–614, 1995.
- A. Corma and A. Martinez, “Zeolites and Zeotypes as catalysts,” Advanced Materials, vol. 7, pp. 137–144, 1995.
- J. Weitkamp and S. Ernst, “Large pore molecular sieves: chapter 5 catalytic test reactions for probing the pore width of large and super-large pore molecular sieves,” Catalysis Today, vol. 19, no. 1, pp. 107–149, 1994.
- W. W. Kaeding, C. Chu, L. B. Young, B. Weinstein, and S. A. Butter, “Selective alkylation of toluene with methanol to produce para-Xylene,” Journal of Catalysis, vol. 67, no. 1, pp. 159–174, 1981.
- R. A. Anderson, “Molecular Sieve Adsorbent Applications State of the Art,” in Molecular Sieves-II, vol. 40 of ACS Symposium Series, chapter 53, pp. 637–649, 1977.
- E. M. Flanigen, “Molecular sieve zeolite technology: the first twenty-five years,” in Proceedings of the Properties and Applications of Zeolites, p. 760, Naples, Italy, 1980.
- D. B. Broughton, “Bulk separations via adsorptions,” Chemical Engineering Progress, vol. 73, p. 49, 1977.
- H. Odawara, Y. Noguchi, and M. Ohno, “Fructose is effectively separated from a mixture of sugars by contacting an aqueous solution of a mixture of sugars with crystalline alumino-silicate,” US Patent 4014711, 1977.
- R. W. Neuziland and J. W. Preighitz, US Patent 4024331, 1977.
- H. Minato and T. Tamura, Natural Zeolites: Ocurrence, Properties and Use, Pergamon, London, UK, 1978.
- J. Nováková and Z. Dolejšek, “A comment on the oxidation of coke deposited on zeolites,” Zeolites, vol. 10, no. 3, pp. 189–192, 1990.
- A. P. Antunes, M. F. Ribeiro, J. M. Silva, F. R. Ribeiro, P. Magnoux, and M. Guisnet, “Catalytic oxidation of toluene over CuNaHY zeolites coke formation and removal,” Applied Catalysis B, vol. 33, no. 2, pp. 149–164, 2001.
- A. P. Bolton, Experimental Methods in Catalytic Research, vol. 2, Academic Press, New York, NY, USA, 1976.
- E. M. Flanigen, “Zeolites, science and technology,” in Proceedings of the NATO ASI, F. R. Ribeiro, Ed., p. 4, Atinus Nijhoff, 1984.
- H. W. Haynes, “Chemical, physical, and catalytic properties of large pore acidic zeolites,” Catalysis Reviews, vol. 17, no. 2, pp. 273–336, 1978.
- E. M. Flanigen, R. W. Broach, and S. T. Wilson, Introduciton, Zeolites in Industrial Separation and Catalysis, Wiley-VCH, Weinheim, Germany, 2010.
- H. Beyer and I. Belenykaja, Catalyisis by the Zeolites, Edited by Y. Imelik, Elsevier, Amsterdam, The Netherlands, 1987.
- J. Scherzer and J. L. Bass, “Infrared spectra of ultrastable zeolites derived from type Y zeolites,” Journal of Catalysis, vol. 28, no. 1, pp. 101–115, 1973.
- N. Y. Chen, “Hydrophobic properties of zeolites,” The Journal of Physical Chemistry, vol. 80, no. 1, pp. 60–64, 1976.
- E. M. Flanigen, J. M. Bennett, R. W. Grose et al., “Silicalite, a new hydrophobic crystalline silica molecular sieve,” Nature, vol. 271, no. 5645, pp. 512–516, 1978.
- E. M. Flanigen and R. L. Patton, “Silica polymorph and process for preparing same,” US Patent 4073865, 1978.
- D. W. Breck, Zeolite Molecular Sieves, Structure, Chemistry and Use, John Wiley & Sons, New York, NY, USA, 1974.
- R. M. Barret, Zeolites and Clay Minerals As Sorbents and Molecular Sieves, Academic Press, London, UK, 1978.
- D. W. Breck, Zeolite Molecular Sieves, Wiley, New York, NY, USA, 1974.
- J. Scherzer, J. L. Bass, and F. G. Hunter, “Structural characterization of hydrothermally treated lanthanum Y zeolites. I. Framework vibrational spectra and crystal structure,” The Journal of Physical Chemistry, vol. 79, no. 12, pp. 1194–1199, 1975.
- P. B. Venuto, L. A. Hamilton, and P. S. Landis, “Organic reactions catalyzed by crystalline aluminosilicates: II. Alkylation reactions: mechanistic and aging considerations,” Journal of Catalysis, vol. 5, no. 3, pp. 484–493, 1996.
- J. W. Ward, “Spectroscopic study of the surface of zeolite Y. II. Infrared spectra of structural hydroxyl groups and adsorbed water on alkali, alkaline earth, and rare earth ion-exchanged zeolites,” The Journal of Physical Chemistry, vol. 72, no. 12, pp. 4211–4223, 1968.
- J. Scherzer, J. L. Bass, and F. G. Hunter, “Structural characterization of hydrothermally treated lanthanum Y zeolites. I. Framework vibrational spectra and crystal structure,” The Journal of Physical Chemistry, vol. 79, no. 12, pp. 1194–1199, 1975.
- G. A. Ozin, A. Kuperman, and A. Stein, “Advanced zeolite, materials science,” Angewandte Chemie, vol. 28, no. 3, pp. 359–376, 1989.
- Z. Wang, A. Mitra, H. Wang, L. Huang, and Y. Yan, “Pure-silica zeolite low-k dielectric thin films,” Advanced Materials, vol. 13, no. 10, pp. 746–749, 2001.
- European Communities Office for Official Publications, Hydrogen and electricity. New carriers and novel technologies for a future clean and sustainable energy economy. EU Brochure for the Sixth Framework Programme. KI-46-02-533-EN-D, 2002.
- M. A. Peña, J. P. Gomez, and G. J. L. Fierro, “New catalytic routes for syngas and hydrogen production,” Applied Catalysis A, vol. 144, no. 1-2, pp. 7–57, 1996.
- J. A. Armor, “The multiple roles for catalysis in the production of H2,” Applied Catalysis A, vol. 176, no. 2, pp. 159–176, 1998.
- D. L. Trimm and Z. I. Onsan, “Onboard fuel conversion for hydrogen-fuel-cell-driven vehicles,” Catalysis Reviews: Science and Engineering, vol. 43, no. 1-2, pp. 31–84, 2001.
- R. M. Navarro, M. A. Peña, and J. L. G. Fierro, “Hydrogen production reactions from carbon feedstocks: fossil fuels and biomass,” Chemical Reviews, vol. 107, no. 10, pp. 3952–3991, 2007.
- T. A. Milne, C. C. Elam, and R. J. Evans, “Hydrogen from biomass,” Report for the International Energy Agency IEA/H2/TR-02/001, 2002.
- P. C. Hallenbeck and J. R. Benemann, “Biological hydrogen production; Fundamentals and limiting processes,” International Journal of Hydrogen Energy, vol. 27, no. 11-12, pp. 1185–1193, 2002.
- D. Gardner, “Hydrogen production from renewables,” Renewable Energy Focus, vol. 9, no. 7, pp. 34–37, 2009.
- G. A. Deluga, J. R. Salge, L. D. Schmidt, and X. E. Verykios, “Renewable hydrogen from ethanol by autothermal reforming,” Science, vol. 303, no. 5660, pp. 993–997, 2004.
- J. R. Salge, B. J. Dreyer, P. J. Dauenhauer, and L. D. Schmidt, “Renewable hydrogen from nonvolatile fuels by reactive flash volatilization,” Science, vol. 314, no. 5800, pp. 801–804, 2006.
- R. M. Navarro, M. C. Sánchez-Sánchez, M. C. Alvarez-Galvan, F. D. Valle, and J. L. G. Fierro, “Hydrogen production from renewable sources: biomass and photocatalytic opportunities,” Energy and Environmental Science, vol. 2, no. 1, pp. 35–54, 2009.
- P. D. Vaidya and A. E. Rodrigues, “Insight into steam reforming of ethanol to produce hydrogen for fuel cells,” Chemical Engineering Journal, vol. 117, no. 1, pp. 39–49, 2006.
- G. Kolios, B. Glöckler, A. Gritsch, A. Morillo, and G. Eigenberger, “Heat-integrated reactor concepts for hydrogen production by methane steam reforming,” Fuel Cells, vol. 5, no. 1, pp. 52–65, 2005.
- A. Haryanto, S. Fernando, N. Murali, and S. Adhikari, “Current status of hydrogen production techniques by steam reforming of ethanol: a review,” Energy and Fuels, vol. 19, no. 5, pp. 2098–2106, 2005.
- M. Ni, D. Y. C. Leung, and M. K. H. Leung, “A review on reforming bio-ethanol for hydrogen production,” International Journal of Hydrogen Energy, vol. 32, no. 15, pp. 3238–3247, 2007.
- G. A. Deluga, J. R. Salge, L. D. Schmidt, and X. E. Verykios, “Renewable hydrogen from ethanol by autothermal reforming,” Science, vol. 303, no. 5660, pp. 993–997, 2004.
- A. N. Fatsikostas and X. E. Verykios, “Reaction network of steam reforming of ethanol over Ni-based catalysts,” Journal of Catalysis, vol. 225, no. 2, pp. 439–452, 2004.
- J. Llorca, P. Ramírez de la Piscina, J. Sales, and N. Homs, “Direct production of hydrogen from ethanolic aqueous solutions over oxide catalysts,” Chemical Communications, no. 7, pp. 641–642, 2001.
- C. Diagne, H. Idriss, and A. Kiennemann, “Hydrogen production by ethanol reforming over Rh/CeO2-ZrO2 catalysts,” Catalysis Communications, vol. 3, no. 12, pp. 565–571, 2002.
- J. Llorca, P. Ramírez De La Piscina, J. A. Dalmon, J. Sales, and N. Homs, “Co-free hydrogen from steam-reforming of bioethanol over ZnO-supported cobalt catalysts: effect of the metallic precursor,” Applied Catalysis B, vol. 43, no. 4, pp. 355–369, 2003.
- E. Vanhaecke, A. C. Roger, J. C. Vargas, and A. Kiennemann, “Challenges & opportunities to bring hydrogen & fuel cells to an international market,” in Proceedings of the1st European Hydrogen Energy Conference, p. 2, Grenoble, France, September 2003.
- M. S. Batista, R. K. S. Santos, E. M. Assaf, J. M. Assaf, and E. A. Ticianelli, “High efficiency steam reforming of ethanol by cobalt-based catalysts,” Journal of Power Sources, vol. 134, no. 1, pp. 27–32, 2004.
- A. Kaddouri and C. Mazzocchia, “A study of the influence of the synthesis conditions upon the catalytic properties of Co/SiO2 or Co/Al2O3 catalysts used for ethanol steam reforming,” Catalysis Communications, vol. 5, no. 6, pp. 339–345, 2004.
- J. Llorca, J. A. Dalmon, P. Ramírez De la Piscina, and N. Homs, “In situ magnetic characterisation of supported cobalt catalysts under steam-reforming of ethanol,” Applied Catalysis A, vol. 243, no. 2, pp. 261–269, 2003.
- F. Haga, T. Nakajima, H. Miya, and S. Mishima, “Catalytic properties of supported cobalt catalysts for steam reforming of ethanol,” Catalysis Letters, vol. 48, no. 1-2, pp. 223–227, 1997.
- H. Idriss, “Ethanol reactions over the surfaces of noble metal/cerium oxide catalysts,” Platinum Metals Review, vol. 48, no. 3, pp. 105–115, 2004.
- J. Bussi, N. Bespalko, S. Veiga, A. Amaya, R. Faccio, and M. C. Abello, “The preparation and properties of Ni-La-Zr catalysts for the steam reforming of ethanol,” Catalysis Communications, vol. 10, no. 1, pp. 33–38, 2008.
- G. B. Sun, K. Hidajat, X. S. Wu, and S. Kawi, “A crucial role of surface oxygen mobility on nanocrystalline Y2O3 support for oxidative steam reforming of ethanol to hydrogen over Ni/Y2O3 catalysts,” Applied Catalysis B, vol. 81, no. 3-4, pp. 303–312, 2008.
- E. B. Pereira, N. Homs, S. Marti, J. L. G. Fierro, and P. R. de la Piscina, “Oxidative steam-reforming of ethanol over Co/SiO2, Co-Rh/SiO2 and Co-Ru/SiO2 catalysts: catalytic behavior and deactivation/regeneration processes,” Journal of Catalysis, vol. 257, no. 1, pp. 206–214, 2008.
- H. V. Fajardo, L. F. D. Probst, N. L. V. Carreno, I. T. S. Garcia, and A. Valentini, “Hydrogen production from ethanol steam reforming over Ni/CeO2 nanocomposite catalysts,” Catalysis Letters, vol. 119, no. 3-4, pp. 228–236, 2007.
- S. Cavallaro, “Ethanol steam reforming on Rh/Al2O3 Catalysts,” Energy and Fuels, vol. 14, no. 6, pp. 1195–1199, 2000.
- M. Tóth, M. Dömök, J. Raskóx, A. Hancz, and A. Erdohelyi, “Catalysts: a comparison between cobalt integration and cobalt. Impregnation,” in Presented in the Technical Program, Pisa, Italy, May 2004.
- V. Fierro, V. Klouz, O. Akdim, and C. Mirodatos, “Oxidative reforming of biomass derived ethanol for hydrogen production in fuel cell applications,” Catalysis Today, vol. 75, no. 1–4, pp. 141–144, 2002.
- S. Velu, N. Satoh, C. S. Gopinath, and K. Suzuki, “Oxidative reforming of bio-ethanol over CuNiZnAl mixed oxide catalysts for hydrogen production,” Catalysis Letters, vol. 82, no. 1-2, pp. 145–152, 2002.
- M. A. Goula, S. K. Kontou, and P. E. Tsiakaras, “Hydrogen production by ethanol steam reforming over a commercial Pd/γ-Al2O3 catalyst,” Applied Catalysis B, vol. 49, no. 2, pp. 135–144, 2004.
- P. Sheng and H. Idriss, “Ethanol reactions over Au-Rh/CeO2 catalysts. Total decomposition and H2 formation,” Journal of Vacuum Science & Technology A, vol. 22, no. 4, article 1652, 7 pages, 2004.
- D. Srinivas, C. V. V. Satyanarayana, H. S. Potdar, and P. Ratnasamy, “Structural studies on NiO-CeO2-ZrO2 catalysts for steam reforming of ethanol,” Applied Catalysis A, vol. 246, no. 2, pp. 323–334, 2003.
- N. R. C. F. Machado, R. C. P. Rizzo, and P. P. S. Peguen, “Performance of catalysts with Nb2O5 for hydrogen production from ethanol steam reforming,” Acta Science, vol. 26, pp. 1637–1642, 2002.
- V. V. Galvita, V. D. Belyaev, V. A. Semikolenov, P. Tsiakaras, A. Frumin, and V. A. Sobyanin, “Ethanol decomposition over Pd-based catalyst in the presence of steam,” Reaction Kinetics and Catalysis Letters, vol. 76, no. 2, pp. 343–351, 2002.
- A. Platon, H. S. Roh, D. L. King, and Y. Wang, “Deactivation studies of Rh/Ce0.8Zr0.2O2 catalysts in low temperature ethanol steam reforming,” Topics in Catalysis, vol. 46, no. 3-4, pp. 374–379, 2007.
- A. Birot, F. Epron, C. Descorme, and D. Duprez, “Ethanol steam reforming over Rh/CexZr1-xO2 catalysts: impact of the CO-CO2-CH4 interconversion reactions on the H2 production,” Applied Catalysis B, vol. 79, no. 1, pp. 17–25, 2008.
- W. Cai, F. Wang, E. Zhan, A. C. Van Veen, C. Mirodatos, and W. Shen, “Hydrogen production from ethanol over Ir/CeO2 catalysts: a comparative study of steam reforming, partial oxidation and oxidative steam reforming,” Journal of Catalysis, vol. 257, no. 1, pp. 96–107, 2008.
- M. Domok, K. Baan, T. Kecskes, and A. Erdohelyi, “Promoting mechanism of potassium in the reforming of ethanol on Pt/Al2O3 Catalyst,” Catalysis Letters, vol. 126, no. 1-2, pp. 49–57, 2008.
- A. C. Bagasiannis, P. Panagiotopoulou, and X. E. Verykios, “Preface,” Topics in Catalysis, vol. 51, no. 1–4, p. 1, 2008.
- J. Llorca, N. Homs, J. Sales, and P. Ramírez de la Piscina, “Efficient production of hydrogen over supported cobalt catalysts from ethanol steam reforming,” Journal of Catalysis, vol. 209, no. 2, pp. 306–317, 2002.
- J. F. da Costa Serra, R. Guil-López, and A. Chica, “Co/ZnO and Ni/ZnO catalysts for hydrogen production by bioethanol steam reforming. Influence of ZnO support morphology on the catalytic properties of Co and Ni active phases,” International Journal of Hydrogen Energy, vol. 13, no. 143, pp. 6709–6716, 2010.
- A. Chica and S. Sayas, “Effective and stable bioethanol steam reforming catalyst based on Ni and Co supported on all-silica delaminated ITQ-2 zeolite,” Catalysis Today, vol. 146, no. 1-2, pp. 37–43, 2009.
- F. C. Campos-Skrobot, R. C. P. Rizzo-Domingues, N. R. C. Fernandes-Machado, and M. P. Cantão, “Novel zeolite-supported rhodium catalysts for ethanol steam reforming,” Journal of Power Sources, vol. 183, no. 2, pp. 713–716, 2008.
- H. Inokawa, S. Nishimoto, Y. Kameshima, and M. Miyake, “Difference in the catalytic activity of transition metals and their cations loaded in zeolite y for ethanol steam reforming,” International Journal of Hydrogen Energy, vol. 35, no. 21, pp. 11719–11724, 2010.
- J. F. da Costa Serra and A. Chica, “Bioethanol steam reforming on Co/ITQ-18 catalyst: effect of the crystalline structure of the delaminated zeolite ITQ-18,” International Journal of Hydrogen Energy, vol. 36, no. 6, pp. 3862–3869, 2011.
- A. Corma, V. Fornes, and U. Dıaz, “ITQ-18 a new delaminated stable zeolite,” Chemical Communications, no. 24, pp. 2642–2643, 2001.
- B. S. Kwak, J. S. Lee, J. S. Lee, B.-H Choi, M. J. Ji, and M. Kang, “Hydrogen-rich gas production from ethanol steam reforming over Ni/Ga/Mg/Zeolite Y catalysts at mild temperature,” Applied Energy, vol. 88, no. 12, pp. 4366–4375, 2011.
- H. Inokawa, S. Nishimoto, Y. Kameshima, and M. Miyake, “Promotion of H2 production from ethanol steam reforming by zeolite basicity,” International Journal of Hydrogen Energy, vol. 36, no. 23, pp. 15195–15202, 2011.
- J. S. Lee, J. Kim, and M. Kang, “Hydrogen production from ethanol steam reforming over SnO2-K2O/zeolite Y catalyst,” Bulletin of the Korean Chemical Society, vol. 32, no. 6, pp. 1912–1920, 2011.
- C. T. Kresge, M. E. Leonowicz, W. J. Roth, J. C. Vartuli, and J. S. Beck, “Ordered mesoporous molecular sieves synthesized by a liquid-crystal template mechanism,” Nature, vol. 359, no. 6397, pp. 710–712, 1992.
- S. Inagaki, Y. Fuhushima, and K. J. Kuroda, “Synthesis of highly ordered mesoporous materials from a layered polysilicate,” Journal of the Chemical Society, Chemical Communications, no. 8, pp. 680–682, 1993.
- Y. Tao, H. Kanoh, L. Abrams, and K. Kaneko, “Mesopore-modified zeolites: preparation, characterization, and applications,” Chemical Reviews, vol. 106, no. 3, pp. 896–910, 2006.
- J. Perez-Ramirez, C. H. Christensen, K. Egeblad, C. H. Christensen, and J. C. Groen, “Hierarchical zeolites: enhanced utilisation of microporous crystals in catalysis by advances in materials design,” CChemical Society Reviews, vol. 37, no. 11, pp. 2530–2542, 2008.
- M. Ogura, “Towards realization of a micro- and mesoporous composite silicate catalyst,” Catalysis Surveys from Asia, vol. 12, no. 1, pp. 16–27, 2008.
- A. Corma, “Application of zeolites in fluid catalytic cracking and related processes,” Studies in Surface Science and Catalysis, vol. 49, pp. 49–67, 1989.
- J. C. Groen, J. A. Moulijn, and J. Pérez-Ramirez, “Desilication: on the controlled generation of mesoporosity in MFI zeolites,” Journal of Materials Chemistry, vol. 16, no. 22, pp. 2121–2131, 2006.
- D. Verboekend and J. Perez-Ramirez, “Design of hierarchical zeolite catalysts by desilication,” Catal. Science & Tecnology, vol. 1, no. 6, pp. 879–890, 2011.
- J. C. Groen, L. A. A. Peffer, J. A. Moulijn, and J. Pérez-Ramírez, “Mesoporosity development in ZSM-5 zeolite upon optimized desilication conditions in alkaline medium,” Colloids and Surfaces A, vol. 24, no. 1–3, pp. 53–58, 2004.
- J. C. Groen, R. Caicedo-Realpe, S. Abelló, and J. Pérez-Ramirez, “Mesoporous metallosilicate zeolites by desilication: on the generic pore-inducing role of framework trivalent heteroatoms,” Materials Letters, vol. 63, no. 12, pp. 1037–1040, 2009.
- Y. Tao, H. Kanoh, and K. Kaneko, “Developments and structures of mesopores in alkaline-treated ZSM-5 zeolites,” Adsorption, vol. 12, no. 5-6, pp. 309–316, 2006.
- M. M. Otten, M. J. Clayton, and H. H. Lamb, “Platinum-mordenite catalysts for n-hexane isomerization: characterization by X-Ray absorption spectroscopy and chemical probes,” Journal of Catalysis, vol. 149, no. 1, pp. 211–222, 1994.
- B. T. Carvill, B. A. Lerner, B. J. Adelman, D. C. Tomazack, and V. M. W. Sachtler, “Increased catalytic activity caused by local destruction of linear zeolite channels: effect of reduction temperature on heptane conversion over platinum supported in H-mordenite,” Journal of Catalysis, vol. 144, no. 1, pp. 1–8, 1993.
- M. S. Holm, E. Taarning, K. Egeblad, and C. H. Christensen, “Catalysis with hierarchical zeolites,” Catalysis Today, vol. 168, no. 1, pp. 3–16, 2011.
- D. H. Park, S. S. Kim, H. Wang et al., “Selective petroleum refining over a zeolite catalyst with small intracrystal mesopores,” Angewandte Chemie, vol. 48, no. 41, pp. 7645–7648, 2009.
- H. J. Park, K. H. Park, J. K. Jeon et al., “Production of phenolics and aromatics by pyrolysis of miscanthus,” Fuel, vol. 97, pp. 379–384, 2012.
- A. J. Foster, J. Jae, Y. T. Cheng, G. W. Huber, and R. F. Lobo, “Optimizing the aromatic yield and distribution from catalytic fast pyrolysis of biomass over ZSM-5,” Applied Catalysis A, vol. 423-424, pp. 154–161, 2012.
- G. T. Neumann and J. C. Hicks, “Novel hierarchical cerium-incorporated MFI zeolite catalysts for the catalytic fast pyrolysis of lignocellulosic biomass,” ACS Catalysis, vol. 2, no. 4, pp. 642–646, 2012.
- M. J. Jeon, S. S. Kim, K. J. Jeon et al., “Catalytic pyrolysis of waste rice husk over mesoporous materials,” Nanoscale Research Letters, vol. 7, article 18, 2012.
- V. Paixao, A. P. Carvalho, J. Rocha, A. Fernandes, and A. Martins, “Modification of MOR by desilication treatments: structural, textural and acidic characterization,” Micro and Mesoporous Materials, vol. 131, no. 1–3, pp. 350–357, 2010.
- J. F. da Costa Serra, M. T. Navarro, F. Rey, and A. Chica, “Bioethanol steam reforming on Ni-based modified mordenite. Effect of mesoporosity, acid sites and alkaline metals,” International Journal of Hydrogen Energy, vol. 37, no. 8, pp. 7101–7108, 2012.
- R. D. Cortright, R. R. Davda, and J. A. Dumesic, “Hydrogen from catalytic reforming of biomass-derived hydrocarbons in liquid water,” Nature, vol. 418, no. 6901, pp. 964–967, 2002.
- R. R. Davda, J. W. Shabaker, G. W. Huber, R. D. Cortright, and J. A. Dumesic, “A review of catalytic issues and process conditions for renewable hydrogen and alkanes by aqueous-phase reforming of oxygenated hydrocarbons over supported metal catalysts,” Applied Catalysis B, vol. 56, no. 1-2, pp. 171–186, 2005.
- G. W. Huber and J. A. Dumesic, “An overview of aqueous-phase catalytic processes for production of hydrogen and alkanes in a biorefinery,” Catalysis Today, vol. 111, no. 1-2, pp. 119–132, 2006.
- Z. Tang, J. Monroe, J. Dong, T. Nenoff, and D. Weinkauf, “Platinum-loaded NaY zeolite for aqueous-phase reforming of methanol and ethanol to hydrogen,” Industrial and Engineering Chemistry Research, vol. 48, no. 5, pp. 2728–2733, 2009.
- N. S. Lewis and D. G. Nocera, “Powering the planet: chemical challenges in solar energy utilization,” Proceedings of the National Academy of Sciences of the United States of America, vol. 103, no. 43, pp. 15729–15735, 2006.
- X. Chen, S. Shen, L. Guo, and S. S. Mao, “Semiconductor-based photocatalytic hydrogen generation,” Chemical Reviews, vol. 110, no. 11, pp. 6503–6570, 2010.
- A. Kudo and Y. Miseki, “Heterogeneous photocatalyst materials for water splitting,” Chemical Society Reviews, vol. 38, no. 1, pp. 253–278, 2009.
- A. Fujishima and K. Honda, “Electrochemical photolysis of water at a semiconductor electrode,” Nature, vol. 238, no. 5358, pp. 37–38, 1972.
- A. Kudo, H. Kato, and I. Tsuji, “Strategies for the development of visible-light-driven photocatalysts for water splitting,” Chemistry Letters, vol. 33, no. 12, pp. 1534–1539, 2004.
- K. Domen, S. Naito, T. Onishi, and K. Tamaru, “Photocatalytic decomposition of liquid water on a NiOSrTiO3 catalyst,” Chemical Physics Letters, vol. 92, no. 4, pp. 433–434, 1982.
- Y. Inoue, T. Kubokawa, and K. Sato, “Photocatalytic activity of sodium hexatitanate, Na2Ti6O13, with a tunnel structure for decomposition of water,” Journal of the Chemical Society, Chemical Communications, no. 19, pp. 1298–1299, 1990.
- T. Takata, Y. Furumi, K. Shinohara et al., “Photocatalytic decomposition of water on spontaneously hydrated layered perovskites,” Chemistry of Materials, vol. 9, no. 5, pp. 1063–1064, 1997.
- A. Kudo, K. Sayama, A. Tanaka et al., “Nickel-loaded K4Nb6O17 photocatalyst in the decomposition of H2O into H2 and O2: structure and reaction mechanism,” Journal of Catalysis, vol. 120, no. 2, pp. 337–352, 1989.
- K. Sayama, A. Tanaka, K. Domen, K. Maruya, and T. Onishi, “Photocatalytic decomposition of water over platinum-intercalated K4Nb6O17,” Journal of Physical Chemistry, vol. 95, no. 3, pp. 1345–1348, 1991.
- A. Kudo and H. Kato, “Photocatalytic decomposition of water into H2 and O2 over novel photocatalyst K3Ta3Si2O13 with pillared structure consisting of three TaO6 chains,” Chemistry Letters, vol. 26, no. 9, pp. 867–868, 1997.
- T. Ishihara, H. Nishiguchi, K. Fukamachi, and Y. Takita, “Effects of acceptor doping to KTaO3 on photocatalytic decomposition of pure H2O,” Journal of Physical Chemistry B, vol. 103, no. 1, pp. 1–3, 1999.
- A. Kudo, H. Kato, and S. Nakagawa, “Water splitting into H2 and O2 on New Sr2M2O7 (M = Nb and Ta) photocatalysts with layered perovskite structures: factors affecting the photocatalytic activity,” The Journal of Physical Chemistry B, vol. 104, no. 3, pp. 571–575, 2000.
- H. Kato and A. Kudo, “Water splitting into H2 and O2 on alkali tantalate photocatalysts ATaO3 (A = Li, Na, and K),” The Journal of Physical Chemistry B, vol. 105, no. 19, pp. 4285–4292, 2001.
- A. Kudo, K. Asakura, and H. Kato, “Highly eficient water splitting into H2 and O2 over lanthanum-doped NaTaO3 photocatalysts with high crystallinity and surface nanostructure,” Journal of the American Chemical Society, vol. 125, no. 10, pp. 3082–3089, 2003.
- Z. Zou, J. Ye, K. Sayama, and H. Arakawa, “Direct splitting of water under visible light irradiation with an oxide semiconductor photocatalyst,” Nature, vol. 414, no. 6864, pp. 625–627, 2001.
- M. Machida, J. I. Yabunaka, and T. Kijima, “Synthesis and photocatalytic property of layered perovskite tantalates, RbLnTa2O7 (Ln = La, Pr, Nd, and Sm),” Chemistry of Materials, vol. 12, no. 3, pp. 812–817, 2000.
- H. Kato and A. Kudo, “Visible-light-response and photocatalytic activities of TiO2 and SrTiO3 photocatalysts codoped with antimony and chromium,” The Journal of Physical Chemistry B, vol. 106, no. 19, pp. 5029–5034, 2002.
- T. Ishii, H. Kato, and A. Kudo, “H2 evolution from an aqueous methanol solution on SrTiO3 photocatalysts codoped with chromium and tantalum ions under visible light irradiation,” Journal of Photochemistry and Photobiology A, vol. 163, no. 1-2, pp. 181–186, 2004.
- I. Tsuji, H. Kato, H. Kobayashi, and A. Kudo, “Photocatalytic H2 evolution reaction from aqueous solutions over band structure-controlled (AgIn)xZn2(1-x)S2 solid solution photocatalysts with visible-light response and their surface nanostructures,” Journal of the American Chemical Society, vol. 126, no. 41, pp. 13406–13413, 2004.
- I. Tsuji, H. Kato, and A. Kudo, “Photocatalytic hydrogen evolution on ZnS−CuInS2−AgInS2 solid solution photocatalysts with wide visible light absorption bands,” Chemistry of Materials, vol. 18, no. 7, pp. 1969–1975, 2006.
- D. Yamasita, T. Takata, M. Hara, J. N. Kondo, and K. Domen, “Recent progress of visible-light-driven heterogeneous photocatalysts for overall water splitting,” Solid State Ionics, vol. 172, no. 1–4, pp. 591–595, 2004.
- R. Niishiro, H. Kato, and A. Kudo, “Nickel and either tantalum or niobium-codoped TiO2 and SrTiO3 photocatalysts with visible-light response for H2 or O2 evolution from aqueous solutions,” Physical Chemistry Chemical Physics, vol. 7, no. 10, pp. 2241–2245, 2005.
- I. Tsuji and A. Kudo, “H2 evolution from aqueous sulfite solutions under visible-light irradiation over Pb and halogen-codoped ZnS photocatalysts,” Journal of Photochemistry and Photobiology A, vol. 156, no. 1–3, pp. 249–252, 2003.
- O. Diwald, T. L. Thompson, E. G. Goralski, S. D. Walck, and J. T. Yates, “The effect of nitrogen ion implantation on the photoactivity of TiO2 rutile single crystals,” Journal of Physical Chemistry B, vol. 108, no. 1, pp. 52–57, 2004.
- R. Konta, T. Ishii, H. Kato, and A. Kudo, “Photocatalytic activities of noble metal ion doped SrTiO3 under visible light irradiation,” Journal of Physical Chemistry B, vol. 108, no. 26, pp. 8992–8995, 2004.
- I. Tsuji, H. Kato, and A. Kudo, “Visible-light-induced H2 evolution from an aqueous solution containing sulfide and sulfite over a ZnS-CuInS2-AgInS2 solid-solution photocatalyst,” Angewandte Chemie, vol. 44, no. 23, pp. 3565–3568, 2005.
- T. L. Thompson and J. T. Yates, “Surface science studies of the photoactivation of TiO2 new photochemical processes,” Chemical Reviews, vol. 106, no. 10, pp. 4428–4453, 2006.
- J. L. Gole, J. D. Stout, C. Burda, Y. Lou, and X. Chen, “Highly efficient formation of visible light tunable TiO2-xNx photocatalysts and their transformation at the nanoscale,” Journal of Physical Chemistry B, vol. 108, no. 4, pp. 1230–1240, 2004.
- C. Di Valentin, G. Pacchioni, and A. Selloni, “Origin of the different photoactivity of N-doped anatase and rutile TiO2,” Physical Review B, vol. 70, Article ID 18202, 4 pages, 2004.
- G. Hitoki, A. Ishikawa, T. Takata, J. N. Kondo, M. Hara, and K. Domen, “Ta3N5 as a novel visible light-driven photocatalyst (λ < 600 nm),” Chemistry Letters, no. 7, pp. 736–737, 2002.
- A. Kasahara, K. Nukumizu, G. Hitoki et al., “Photoreactions on LaTiO2N under visible light irradiation,” Journal of Physical Chemistry A, vol. 106, no. 29, pp. 6750–6753, 2002.
- H. Kato, K. Asakura, and A. Kudo, “Highly efficient water splitting into H2 and O2 over Lanthanum-Doped NaTaO3 photocatalysts with high crystallinity and surface nanostructure,” Journal of the American Chemical Society, vol. 125, no. 10, pp. 3082–3089, 2003.
- W. Shangguan and A. Yoshida, “Photocatalytic hydrogen evolution from water on nanocomposites incorporating cadmium sulfide into the interlayer,” Journal of Physical Chemistry B, vol. 106, no. 47, pp. 12227–12230, 2002.
- A. Koca and M. Sahin, “Photocatalytic hydrogen production by direct sun light from sulfide/sulfite solution,” International Journal of Hydrogen Energy, vol. 27, no. 4, pp. 363–367, 2002.
- G. Milczarek, A. Kasuya, S. Mamykin, T. Arai, K. Shinoda, and K. Tohji, “Optimization of a two-compartment photoelectrochemical cell for solar hydrogen production,” International Journal of Hydrogen Energy, vol. 28, no. 9, pp. 919–926, 2003.
- J. R. Plunkett and United States, Energy Information Administration, International Energy Outlook and Projections, Nova Science, Hauppauge, NY, USA, 2011.
- A. Kudo and Y. Miseki, “Heterogeneous photocatalyst materials for water splitting,” Chemical Society Reviews, vol. 38, no. 1, pp. 253–278, 2009.
- M. Ni, M. K. H. Leung, D. Y. C. Leung, and K. Sumathy, “A review and recent developments in photocatalytic water-splitting using TiO2 for hydrogen production,” Renewable and Sustainable Energy Reviews, vol. 11, no. 3, pp. 401–425, 2007.
- M. Matsuoka, M. Kitano, M. Takeuchi, K. Tsujimaru, M. Anpo, and J. M. Thomas, “Photocatalysis for new energy production. Recent advances in photocatalytic water splitting reactions for hydrogen production,” Catalysis Today, vol. 122, no. 1-2, pp. 51–61, 2007.
- T. Bak, J. Nowotny, M. Rekas, and C. C. Sorrell, “Photo-electrochemical hydrogen generation from water using solar energy. Materials-related aspects,” International Journal of Hydrogen Energy, vol. 27, no. 10, pp. 991–1022, 2002.
- Y. A. Shaban and S. U. M. Khan, “Visible light active carbon modified n-TiO2 for efficient hydrogen production by photoelectrochemical splitting of water,” International Journal of Hydrogen Energy, vol. 33, no. 4, pp. 1118–1126, 2008.
- H. Y. Lin, T. H. Lee, and C. Y. Sie, “Photocatalytic hydrogen production with nickel oxide intercalated K4Nb6O17 under visible light irradiation,” International Journal of Hydrogen Energy, vol. 33, no. 15, pp. 4055–4063, 2008.
- H. Y. Lin, Y. F. Chen, and Y. W. Chen, “Water splitting reaction on NiO/InVO4 under visible light irradiation,” International Journal of Hydrogen Energy, vol. 32, no. 1, pp. 86–92, 2007.
- P. S. Lunawat, S. Senapati, R. Kumar, and N. M. Gupta, “Visible light-induced splitting of water using CdS nanocrystallites immobilized over water-repellant polymeric surface,” International Journal of Hydrogen Energy, vol. 32, no. 14, pp. 2784–2790, 2007.
- M. Sathish, B. Viswanathan, and R. P. Viswanath, “Alternate synthetic strategy for the preparation of CdS nanoparticles and its exploitation for water splitting,” International Journal of Hydrogen Energy, vol. 31, no. 7, pp. 891–898, 2006.
- N. Koriche, A. Bouguelia, A. Aider, and M. Trari, “Photocatalytic hydrogen evolution over delafossite CuAlO2,” International Journal of Hydrogen Energy, vol. 30, no. 7, pp. 693–699, 2005.
- J. Ye, Z. Zou, and A. Matsushita, “A novel series of water splitting photocatalysts NiM2O6 (M = Nb, Ta) active under visible light,” International Journal of Hydrogen Energy, vol. 28, no. 6, pp. 651–655, 2003.
- Y. Bessekhouad and M. Trari, “Photocatalytic hydrogen production from suspension of spinel powders AMn2O4(A = Cu and Zn),” International Journal of Hydrogen Energy, vol. 27, no. 4, pp. 357–362, 2002.
- P. K. Dutta and W. Turbeville, “Intrazeolitic photoinduced redox reactions between Ru(bpy)32+ and methylviologen,” Journal of Physical Chemistry, vol. 96, no. 23, pp. 9410–9416, 1992.
- H. Yamashita, Y. Fujii, Y. Ichihashi et al., “Selective formation of CH3OH in the photocatalytic reduction of CO2 with H2O on titanium oxides highly dispersed within zeolites and mesoporous molecular sieves,” Catalysis Today, vol. 45, no. 1–4, pp. 221–227, 1998.
- M. Anpo, H. Yamashita, Y. Ichihashi, Y. Fujii, and M. Honda, “Photocatalytic reduction of CO2 with H2O on titanium oxides anchored within micropores of zeolites: effects of the structure of the active sites and the addition of Pt,” Journal of Physical Chemistry B, vol. 101, no. 14, pp. 2632–2636, 1997.
- S. G. Zhang, Y. Fujii, H. Yamashita, K. Koyano, T. Tatsumi, and M. Anpo, “Photocatalytic reduction of CO2 with H2O on Ti-MCM-41 and Ti-MCM-48 mesoporous zeolites at 328 K,” Chemistry Letters, no. 7, pp. 659–660, 1997.
- M. Anpo, M. Matsuoka, Y. Shioya et al., “Preparation and characterization of the Cu+/ZSM-5 catalyst and its reaction with NO under UV irradiation at 275 K. In situ photoluminescence, EPR, and FT-IR investigations,” Journal of Physical Chemistry, vol. 98, no. 22, pp. 5744–5750, 1994.
- M. Anpo and H. Yamashita, “Photochemistry of surface species anchored on solid surfaces,” in Surface Photochemistry, M. Anpo, Ed., p. 117, Wiley, London, UK, 1996.
- H. Yamashita, Y. Ichihashi, M. Anpo, M. Hashimoto, C. Louis, and M. Che, “Photocatalytic decomposition of NO at 275 K on titanium oxides included within Y-zeolite cavities: the structure and role of the active sites,” The Journal of Physical Chemistry, vol. 100, no. 40, pp. 16041–16044, 1996.
- H. Chen, A. Matsumoto, N. Nishimiya, and K. Tsutsumi, “Preparation and characterization of TiO2 incorporated Y-zeolite,” Colloids and Surfaces A, vol. 157, no. 1–3, pp. 295–305, 1999.
- X. Liu, K. K. Lu, and J. K. Thomas, “Encapsulation of TiO2 in zeolite Y,” Chemical Physics Letters, vol. 195, no. 2-3, pp. 163–168, 1992.
- X. Liu, K. K. Lu, and J. K. Thomas, “Preparation, characterization and photoreactivity of titanium(IV) oxide encapsulated in zeolites,” Journal of the Chemical Society, vol. 89, pp. 1861–1865, 1993.
- Y. Kim and M. Yoon, “TiO2/Y-Zeolite encapsulating intramolecular charge transfer molecules: a new photocatalyst for photoreduction of methyl orange in aqueous medium,” Journal of Molecular Catalysis A, vol. 168, no. 1-2, pp. 257–263, 2000.
- X. Chen and S. S. Mao, “Titanium dioxide nanomaterials: synthesis, properties, modifications, and applications,” Chemical Reviews, vol. 107, no. 7, pp. 2891–2959, 2007.
- S. Ikeda, A. Tanaka, K. Shinohara et al., “Effect of the particle size for photocatalytic decomposition of water on Ni-loaded K4Nb4O17,” Microporous Materials, vol. 9, no. 5-6, pp. 253–258, 1997.
- M. C. Hidalgo, M. Aguilar, M. Maicu, J. A. Navío, and G. Colón, “Hydrothermal preparation of highly photoactive TiO2 nanoparticles,” Catalysis Today, vol. 129, no. 1-2, pp. 50–58, 2007.
- A. Testino, I. R. Bellobono, V. Buscaglia et al., “Optimizing the photocatalytic properties of hydrothermal TiO2 by the control of phase composition and particle morphology. A systematic approach,” Journal of the American Chemical Society, vol. 129, no. 12, pp. 3564–3575, 2007.
- A. Datta, A. Priyam, S. N. Bhattacharyya, K. K. Mukherjea, and A. Saha, “Temperature tunability of size in CdS nanoparticles and size dependent photocatalytic degradation of nitroaromatics,” Journal of Colloid and Interface Science, vol. 322, no. 1, pp. 128–135, 2008.
- S. Y. Chae, M. K. Park, S. K. Lee, T. Y. Kim, S. K. Kim, and W. I. Lee, “Preparation of size-controlled TiO2 nanoparticles and derivation of optically transparent photocatalytic films,” Chemistry of Materials, vol. 15, no. 17, pp. 3326–3331, 2003.
- G. Liu, C. Sun, H. G. Yang et al., “Nanosized anatase TiO2 single crystals for enhanced photocatalytic activity,” Chemical Communications, vol. 46, no. 5, pp. 755–757, 2010.
- Y. Lee, T. Watanabe, T. Takata, M. Hara, M. Yoshimura, and K. Domen, “Hydrothermal synthesis of fine NaTaO3 powder as a highly efficient photocatalyst for overall water splitting,” Bulletin of the Chemical Society of Japan, vol. 80, no. 2, pp. 423–428, 2007.
- Z. Zhang, C. C. Wang, R. Zakaria, and J. Y. Ying, “Role of particle size in nanocrystalline TiOi-based photocatalysts,” Journal of Physical Chemistry B, vol. 102, no. 52, pp. 10871–10878, 1998.
- W. Sun, S. Zhang, Z. Liu, C. Wang, and Z. Mao, “Studies on the enhanced photocatalytic hydrogen evolution over Pt/PEG-modified TiO2 photocatalysts,” International Journal of Hydrogen Energy, vol. 33, no. 4, pp. 1112–1117, 2008.
- D. W. Bahnemann, C. Kormann, and M. R. Hoffmann, “Preparation and characterization of quantum size zinc oxide: a detailed spectroscopic study,” Journal of Physical Chemistry, vol. 91, no. 14, pp. 3789–3798, 1987.
- A. J. Hoffman, E. R. Carraway, and M. R. Hoffmann, “Photocatalytic production of H2O2 and organic peroxides on quantum-sized semiconductor colloids,” Environmental Science & Technology, vol. 28, no. 5, pp. 776–785, 1994.
- A. J. Hoffman, G. Mills, H. Yee, and M. R. Hoffmann, “Q-sized cadmium sulfide: synthesis, characterization, and efficiency of photoinitiation of polymerization of several vinylic monomers,” The Journal of Physical Chemistry, vol. 96, no. 13, pp. 5546–5552, 1992.
- A. J. Hoffman, H. Yee, G. Mills, and M. R. Hoffmann, “Q-sized cadmium sulfide: synthesis, characterization, and efficiency of photoinitiation of polymerization of several vinylic monomers,” The Journal of Physical Chemistry, vol. 96, no. 13, pp. 5540–5552, 1992.
- M. A. Fox and T. L. Pettit, “Photoactivity of zeolite-supported cadmium sulfide: hydrogen evolution in the presence of sacrificial donors,” Langmuir, vol. 5, no. 4, pp. 1056–1061, 1989.
- M. Warrier, M. K. F. Lo, H. Monbouquette, and M. A. Garcia-Garibay, “Photocatalytic reduction of aromatic azides to amines using CdS and CdSe nanoparticles,” Photochemical and Photobiological Sciences, vol. 3, no. 9, pp. 859–863, 2004.
- M. Sathish, B. Vishwanathan, and R. P. Vishwanath, “Alternate synthetic strategy for the preparation of CdS nanoparticles and its exploitation for water splitting,” International Journal of Hydrogen Energy, vol. 31, no. 7, pp. 891–898, 2006.
- S. Y. Ryu, W. Balcerski, T. K. Lee, and M. R. Hoffmann, “Photocatalytic production of hydrogen from water with visible light using hybrid catalysts of CdS attached to microporous and mesoporous silicas,” Journal of Physical Chemistry C, vol. 111, no. 49, pp. 18195–18203, 2007.
- S. Y. Ryu, J. Choi, W. Balcerski, T. K. Lee, and M. R. Hoffmann, “Photocatalytic production of H2 on nanocomposite catalysts,” Industrial and Engineering Chemistry Research, vol. 46, no. 23, pp. 7476–7488, 2007.
- P. Yue and F. Khan, “Methods for increasing photo-assisted production of hydrogen over titanium exchanged zeolites,” International Journal of Hydrogen Energy, vol. 16, no. 9, pp. 609–613, 1991.
- G. Guan, T. Kida, K. Kusakabe, K. Kimura, X. Fang, and T. Ma, “Photocatalytic H2 evolution under visible light irradiation on CdS/ETS-4 composite,” Chemical Physics Letters, vol. 385, no. 3-4, pp. 319–322, 2004.
- G. Guan, T. Kida, K. Kusakabe et al., “Photocatalytic H2 evolution under visible light irradiation on CdS/ETS-4 composite,” Chemical Physics Letters, vol. 385, no. 3-4, pp. 319–322, 2004.
- N. Dubey, S. S. Rayalu, N. K. Labhsetwar, and S. Devotta, “Visible light active zeolite-based photocatalysts for hydrogen evolution from water,” International Journal of Hydrogen Energy, vol. 33, no. 21, pp. 5958–5966, 2008.
- J. C. White and P. K. Dutta, “Assembly of nanoparticles in zeolite Y for the photocatalytic generation of hydrogen from water,” The Journal of Physical Chemistry C, vol. 115, no. 7, pp. 2938–2947, 2011.
Copyright © 2013 Antonio Chica. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.